Active Standard ASTM D7113 / D7113M | Developed by Subcommittee: D04.21
Book of Standards Volume: 04.03
Historical (view previous versions of standard)
Significance and Use
The test method described is useful as a rapid, nondestructive technique for determining the in-place density or relative compaction of compacted bituminous mixtures.
The test method can be used to establish the proper rolling effort and pattern to achieve the required density.
The non-destructive nature of the test allows repetitive measurements to be made at a single test location between roller passes or at multiple locations across the mat to monitor changes in density.
The density results obtained by this test method are relative. Device calibration (correlation with other test methods] is required to convert the results obtained using this method to actual density. Section 6 of this test method describes a method that has proven to be acceptable for correlation.
Note 1—The personnel and equipment used in performing this test can be evaluated in accordance with Specification D3666.
Note 2—Research and evaluation of devices used in this test method has been conducted. Reference is made to “Evaluation of Non-Nuclear Gauges to Measure Density of Hot-Mixed Asphalt Pavements,” a pooled fund study, Pedro Romero, Ph.D., P.E., July 2002.
1.1 This test method covers the procedures for determining the in-place density and relative compaction of bituminous concrete pavement paving mixtures by an electromagnetic surface contact device by measuring changes in the electromagnetic field resulting from the compaction process.
1.2 The equipment referenced in this method is a surface contact device, which must accommodate surface moisture and temperature variation in the range typically encountered in paving applications. This can be accomplished by design parameters that reduce the device’s sensitivity to surface moisture and temperature variation or by measurements and algorithms to account for surface moisture and temperature variance in the rolling pattern.
1.3 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C670 Practice for Preparing Precision and Bias Statements for Test Methods for Construction Materials
D1188 Test Method for Bulk Specific Gravity and Density of Compacted Bituminous Mixtures Using Coated Samples
D2726 Test Method for Bulk Specific Gravity and Density of Non-Absorptive Compacted Bituminous Mixtures
D3665 Practice for Random Sampling of Construction Materials
D3666 Specification for Minimum Requirements for Agencies Testing and Inspecting Road and Paving Materials
D5361 Practice for Sampling Compacted Bituminous Mixtures for Laboratory Testing
D6752 Test Method for Bulk Specific Gravity and Density of Compacted Bituminous Mixtures Using Automatic Vacuum Sealing Method
ICS Number Code 93.080.20 (Road construction materials)
UNSPSC Code 30121500(Bituminous derivatives)